DRAFT Fine Ceramic Products INTRODUCTION Scope and Relationship to Traditional Ceramic Products Fine ceramics are products that men and women encounter in their everyday lives. These products include ceramic dishes, toilets, tile, and related products. All of these products have in common the use of clay minerals in their composition, and the products have been processed at high temperatures to cause limited melting or fusion producing a glass phase creating a permanent bond within the articles. It is this glass phase, or vitrification, that produces permanence and utility in the products. Ceramic products are those composed of non-metallic and inorganic constituents. In other words, ceramics are composed of metal compounds such as oxides, and traditional ceramics have constituents that commonly occur in the earths crust. This means that traditional ceramics contain oxides of aluminum, silicon, magnesium, calcium, iron, and alkali metals (sodium and potassium) along with trace quantities of other elements. Fine ceramics are those that are essentially made from fine particles, with particle size essentially less than about 150 microns () and typically less than 75 microns. After heating (also known as firing), such ceramics have a fine texture meaning the solid material contains very small crystals and pores of small diameter with crystal size and pore size (diameter) less than the diameter of the starting particulate matter that comprised the ceramic mass. By contrast, traditional ceramics made from large or coarse particles ranging in size up to about 6000 microns include such products as clay bricks, clay roofing tile, refractory bricks, and clay pipe. While coarse particulate ceramics are typically fired in kilns or furnaces to achieve permanence, they generally exhibit lower strength than fine ceramic products. Another important distinction is that many coarse particulate ceramics contain iron oxide in their composition in the range 2-8% by weight producing colors in the fired products ranging from pink to red to blue or black.
Technologists apply the name whitewares to most fine ceramic products, and the term simply reflects the fact that most of the products are white (or near white) in color where ware is the technical name for a ceramic object that is sold in commerce. Under the name whiteware, three are many different functional products (Table 1). Whitewares are usually distinguished or classified in commerce according to these technical subgroups. The classifications usually are distinguished by the amount of void space in the fired ceramic called its porosity. In the historical development of traditional ceramics, porosity was measured indirectly as water absorption, i.e. the weight of water the ceramic would absorb on immersion in water compared to the dry weight of the ceramic object expressed as a percentage of the dry weight. The general relationship in whitewares is that low porosities are associated with high mechanical strength, high resistance to chippage (or breakage), and excellent durability. Adjusting the composition or mineral constitution and increasing the amount or degree of vitrification in firing achieves low porosity in whitewares. With respect to composition, mixtures of clay, flint (ground silica), and feldspar minerals have been found to achieve the highest strengths of clay based-whitewares, and these products are called triaxial whitewares: due to the three components in their composition. Further improvements in strength are noted when aluminum oxide (alumina) and/or other minerals, such as zircon, are added to the composition. Vitrification is achieved in kilns as the ceramic composition melts as temperatures achieve red heat, i.e. rise above about 950oC. As temperature is further increases, more melted phase is formed, and this glass is distributed by capillary forces throughout the ceramic. As temperatures generally increase above 1000oC, a new mineral named mullite appears. Simultaneously, the ceramic ware exhibits shrinkage effectively increasing density and reducing porosity. After cooling in the kiln, the fired product has mechanical properties reflecting the degree of vitrification and densification achieved in the firing process. The degree of vitrification is the percentage of melting of the original constituents that has occurred in manufacturing. In whiteware ceramics, the amount of melting may be as high as 40-60% while in glass products the
extent of melted phase approaches 100%. In manufacturing of whitewares, measurements of firing shrinkage and porosity (water absorption) reflect the quality of the fired product. Table 1: Classification of Unglazed Ceramic Whiteware Products Class Earthenware Stoneware Description Clay based ceramic ware of medium porosity. Ceramics made form a single clay or clay blend with other minerals (including silica) fired to produce a harder and more durable product. Product classes include: Hotel china Bone china Frit china Vitreous plumbing fixtures Cookware Product classes include: Hard porcelain Vitreous porcelain Electrical porcelain Dental porcelain Product classes include: Steatite ceramics Electrical ceramics Distinguishing Factor for this Class Water absorption of 4-20%. Earthenware is typically off-white to red in color due to its iron content. Water absorption 0-5%. Stoneware is typically off-white to gray in color due to its iron content and the presence of non-clay minerals. All product classes typically exhibit water absorption of less than 0.5% except for cookware, which may exhibit up to 5% absorption. The low water absorption creates high strength and minimal water transmission in use. The products may be compositions of flint (quartz), clay, and feldspar (a vitrification enhancer), and they may contain additional minerals to increase their strength (such as aluminum oxide). Steatite ceramics contain the mineral talc to enhance the product performance in high frequency electrical applications. Electrical ceramics usually are porcelains of high aluminum oxide content (such as spark plug insulators). Compositions are altered to include aluminum oxide, zircon, and other minerals to obtain specific properties.
Technical Whiteware Ceramics
This general classification includes many low absorption ceramics for structural and chemical applications.
Whiteware products are typically glazed in order to increase their utility and improve their appearance. A glaze is a glass coating over the ceramic surface formed by melting or fusing a coating that has been applied to all or part of the ceramic wares surface. Glazes provide a smooth surface that can easily be cleaned. Glazes also prevent water to be absorbed by the
product thereby promoting sanitation and/or improving performance. Glazes also can be colored using pigmenting oxides providing enhanced appearance. One advantage of glazing over a white surface is that is it relatively easy to achieve light colors without bleed through of color from the substrate. This is a distinct advantage of whiteware products as compared to red clay (red body) ceramics. With red clay ceramics, it is frequently necessary to apply double layers of glaze (a white under glaze layer topped by a colored outer layer) to achieve a desired light color. Raw Materials for Fine Ceramics and Reactions on Firing Raw materials introduction. A variety of raw materials are used in the production of whiteware ceramics. These raw materials or minerals can generally be broken down into three categories, which are clay, flux and fillers (or non-plastics). Each material has a specific function, but in general, the clay is the component that provides plasticity or cohesion for forming, while the flux promotes vitrification. The filler is typically inert, but it also may serve to modify the glass viscosity during vitrification, which effectively extends the range of firing temperatures of the composition. The component that receives the most attention in traditional ceramic compositions is the clay. Clay is a hydrous sheet silicate that is a product of the weathering of feldspathic parent rock. Clays are defined by their plasticity when mixed with water, and they exhibit an extremely small particle size in an unagglomerated state. A typical particle size distribution is given in Figure 1. This small particle size and the plate like morphology of the particles give rise to a large surface area. Thus, the particle surfaces tend to have an affinity for water. The clay's affinity for water gives rise to a monolayer of water around the particle. The water layer promotes cohesion and allows the particles to slip relative to one another during plastic forming.
Cummulative Percent Finer Than (%)
60 Ball Clay Kaolin 40
Equivalent Spherical Diameter (m)
Figure 1 Typical Clay Particle Size Distribution Since clays are the product of weathering of the parent feldspathic rock, they can exist as either primary (residual) deposits or secondary (sedimentary) deposits. Primary deposits are formed by geological processes in situ, and they typically have the largest particle size and lowest impurity level amongst clay sources. Secondary deposits of clay involved transportation of minerals by water with eventual deposition in the location where they are mined. Secondary deposits typically have smaller particle sizes and higher impurity levels when compared to primary deposits. Being a product of weathering, clays are capable of a wide range of atomic substation in the silicate structure, which gives rise to the large variety of clay minerals. Clays, particularly secondary deposits, also contain non-clay impurities or accessory minerals. The major accessory mineral found with clay deposits is crystalline